**5.5 Cubic nanoplatelets**

**5.5.4 Further study of the dipolar dimensionality**

**5.5.4.1** **Is there any third dipole involved in the emission?**

For nanocrystals and nanoplatelets, the emission is generally modelized to be an one
dimensional dipole or a two dimensional dipole which consists of two orthogonal linear dipolar
components. However, some researchs state that a third dipole orthogonal to the plane of the
two dimensional dipole could play a role in the emission [167,168]. The geometry of the cubic
nanoplatelets gives specific orientations to their emitting dipoles. Then the emission will be
generated from a three dimensional dipole which would be a sum of two dipoles in the platelet
plane and a linear dipole normal to the platelet plane. We could consider these two first dipolar
components having the same oscillator strength. In the case of the platelets which stands on
their side (their core plane is perpendicular to the substrate, as schematized in Figure 5.23), one
of those dipoles is along*z* reference axis and the other is along the (*x, y*) plane. We assume that
a third dipolar contribution exists with relative oscillator strength *η*3 (0 ≤ *η*3 ≤ 1), oriented
perpendicularly to the plane of the other two component dipoles (the core plane), thus it is
also along the (*x, y*) plane, as presented in Figure 5.28. Moreover, as *d*_{3} =*η*_{3}*d*_{1}, when *η*_{3} = 1
this third dipolar component is equivalent to the others while *η*_{3} = 0 means there is no third
dipole.

z d

y

x d2

d_{1}
d_{3}
Φ_{max}

*FIGURE 5.28: Schematic of the emitting dipole of a nanoplatelet standing by its side face.*

**5.5.4.2** **Emission pattern analysis**

We first analyze the data from the lying nanoplatelets in order to see if we could detect
the presence of the third dipolar component. Figure 5.29(b) depicts theoretical emission
pat-tern calculated for a symmetric horizontal two dimensional dipole. We compare it with the
pattern simulated for a three dimensional dipole with *η*_{3} = 1 as presented in Figure 5.29(c).

In both cases, the emitter is at the distance of 50 nm to the PMMA-gold interface and its
emission is collected in the PMMA half-space by an oil objective *N A* =1.4 , as schematized
in Figure 5.29(a). These angular distributions are very similar to each other, so that lying
cubic nanoplatelet do not help us to conclude about the presence of the third component of the
emitting dipole.

*FIGURE 5.29: (a) Schematic of the investigated configuration. Simulated emission pattern of*
*(b) a horizontal symmetric horizontal two dimensional dipole and (c) a three dimentional dipole*
*with* *η*_{3} = 1*.*

We continue performing the emission pattern analysis on the data of the standing cubic
nanoplatetets in the PMMA half-space 50 *nm* to the PMMA-gold interface (5.30(a)). We
cal-culate the emission pattern of a three dimensional dipole with different values of *η*_{3} and plot
their profiles along the in-plane orientation Φ*max* + 90^{o} (blue) and its orthorgonal axis Φ*max*

(green), as depicted in Figure 5.30(c). The experimental values are extracted from the recorded
emission pattern presented in Figure 5.30(b). When *η*_{3} *>*0*.*1, there is a quantitative
disagree-ment between the experidisagree-mental and simulation data. We can conclude that the contribution of
the third dipolar component, if it exists, is less than 10 % of the other dipoles.

**5.5.4.3** **Emission polarization analysis**

Moreover, we could analyze the emission^{0} polarimetric curves which contains more
quan-titative details. We will consider now the experimental results. As stated for *d*_{1} = *d*_{2}, the

-90°

*FIGURE 5.30: (a) Sechematic of the investigated configuration. (b) Experimental emission*
*pattern of a cubic nanoplatelet having its core plane normal to the substrate (c) Comparison of*
*emission patterns along the*Φ*max*+ 90^{o}*(blue) and*Φ*max* *(green) directions: experimental values*
*(dots) and simulated values (lines) with the amplitude of third dipolar componentη*_{3} *is 0.1, 0.2,*
*and 0.5 respectively.*

expected degree of polarization is 0.79. In our data, for one nanoplatelet we obtained *δ*= 0*.*79.

This is the one which has been discussed in the former emission pattern analysis.

As presented in Figure 5.28, this three dimensional dipole is considered as a combination
of a two dimensional dipole of orientation (Θ = *π/*2*,*Φ = *π/*2) which is a sum of two linear
dipoles with the same amplitude, one along (Θ1 = 0*,*Φ1 = 0) and the other oriented at (Θ2 =
*π/*2*,*Φ2 = *π/*2), and a third one dimensional dipole along (Θ3 =*π/*2*,*Φ = 0) of amplitude *η*_{3}
with respect to the 2 others. Thanks to Equation 5.6, we have *P*_{1}^{00}, *P*_{2}^{00} and *P*_{3}^{00} being the total
emitting power contributed by each dipolar components respectively:

*P*_{1}^{00}=*B* (5.23)

*P*_{2}^{00}=*A*+*C* sin^{2}(*β*) (5.24)

*P*_{3}^{00} =*η*_{3}(*A*+*C* cos^{2}(*β*)) (5.25)
The total emission from the three dimensional dipole is thus:

X*P*^{00} =*P*_{1}^{00}+*P*_{2}^{00}+*P*_{3}^{00}

=*B*+*A*+*C*sin^{2}(*β*) +*η*_{3}(*A*+*C* cos^{2}(*β*))

=*A*(*η*_{3}+ 1) +*B* +*Cη*_{3}+*C*(1−*η*_{3}) sin^{2}(*β*)

(5.26)

As 0≤sin^{2}(*β*)≤1 and*η*_{3} ≤1, we have:

*P*_{min}^{00} =*A*(*η*_{3}+ 1) +*B* +*Cη*_{3} (5.27)

*P*_{max}^{00} =*A*(*η*3+ 1) +*B* +*C* (5.28)

The degree of polarization is defined as:

*δ*= *P*_{max}^{00} −*P*_{min}^{00}

*P*_{max}^{00} +*P*_{min}^{00} = *C*(1−*η*_{3})

2*A*(*η*_{3}+ 1) + 2*B*+*C*(*η*_{3}+ 1) (5.29)
Therefore,

*dδ* =− *dη*_{3}

1−*η*_{3} − (2*A*+*C*)*dη*_{3}

2*A*(*η*_{3}+ 1) + 2*B* +*C*(*η*_{3}+ 1) (5.30)
The emitter with *δ* = 0*.*79 (*d*_{1} = *d*_{2}) refers to *η*_{3} = 0. But we need to take into account
the uncertainty of*δ* measurement. Since*η*_{3} ≈0, we have:

*dδ* =−dη_{3}4*A*+ 2*B* + 2*C*

2*A*+ 2*B*+*C* (5.31)

From the data of standing nanoplatelets, we have *dδ* = 0*.*05, leading to *dη*_{3} of 0.03. The
polarimetric measurement allows us to detect the *d*_{3} contribution up to *η*_{3} ≥ 0*.*03. It is thus
concluded that the third dipole if any is less than 3% of the other dipoles.

**Conclusion**

We have studied the emission of an individual colloidal CdSe*/*CdS core*/*shell nanoplatelet.

There are three types of geometric structure: square, rectangle and cube. The ultrathin
nanoplatelets have two different shapes: square (16 x 16 x 2 *nm*^{3}) and rectangle (15 x 20
x 2 *nm*^{3}). The last type of investigated nanoplatelets are cubic (16 x 16 x 10 *nm*^{3}). In this
chapter, we have applied our polarimetric method combined with emission pattern analysis to
determine the emitting dipole of an individual nanoplatelet.

The square nanoplatelets are spincoated on*SiO*_{2} covered gold subtrate then protected by
PMMA layer and their emission is charaterized by an oil objective in contact with PMMA. For
13 studied square nanoplatelets, the emission polarization analysis confirms their unpolarized
emission, resulting in two possible dipolar orientation depending on the one or two dipolar
dimensionality of the emitting dipole. By comparing the calculating emission patterns obtained
by our analytical model with the experimental images for these emitters, we have concluded
that the emitting dipole of the nanoplatelets is a two dimensional dipole with its orientation
along the *z* reference axis.

Analysis on the emission polarization of the rectangular nanoplatelets provides further insight into the emission of these platelets. We found much broader histogram of the degree of polarization which brought to us two different hypotheses for the dipolar orientation: a tilted dipole composed by two degenerate dipoles or a horizontal dipole composed by two non-degenerate dipoles. Using the configuration with only nanoplatelets on glass substrate and the oil objective introduced to the other side of the substrate, the measured Fourier plane image is possible to confirm the latter hypotheses.

The higher degree of polarization obtained by the emission polarization measurement is believed to relate to the elongated shape of these nanoplatelets. The good agreement on extracting the dipolar asymmetric factor from two experimental data set measured by two

different ways (emission polarization characterization and emission pattern imaging) confirm the correlation between two approaching ways. However, since the length of the nanoplatelets is much larger than their exciton Bohr radius, the emitting dipole should not be sensitive to the lateral sizes of nanoplatelets and then could be considered as a symmetric two dimensional dipole. In this case, the polarized emission will be explained by the dielectric antenna effect.

The similarity between emission patterns simulated for an asymmetric two dimensional dipole inside a square nanoplatelet and for a symmetric two dimensional dipole inside a rectangular nanoplatelet confirms the antenna hypothesis.

For cubic nanoplatelets, the same two dipolar dimensionality was found. Most platelets were deposited horizontally on the substrate with their two dipolar components as well hor-izontal, similar to thin shell covered square nanoplatelets. However, in few cases when the nanoplatelets staying on its side face (the core platelet normal to the substrate), their two di-mensional emitting dipole could be considered as having one component horizontal and the other vertical. We consider the possibility of a third dipolar component by analyzing the emission polarization and emission pattern in the case of high polarized emission. Since its contribution is absent or very small, we could conclude that the emitting dipole of these nanoplatelets is just two dimensional.

**Conclusion**

In the stream of various studies to get an efficient source of single-photons, determination of the dipolar orientation of light from a nanoemitter is considered to be very important.

Contribution of my thesis in the field is the development of a polarimetric method aiming at the
analysis of a nanoemitter^{0}s emitting dipole and its orientation. My work includes (i) proposing
an analytical model, (ii) building-in the experiment setup and (iii) applying to determine the
nanoemitter^{0}s emitting dipole.

The model describes the emission of a dipole close to a plane interface in a wide range of
realistic experimental conditions, including a very common case in plasmonics with a
nanoemit-ter lying on gold film, the situation for which the more standard defocused imaging method is
not sufficiently sensitive to provide reliable quantitative information on the emitting dipole^{0}s
orientation. With the same model, I did a computation on the emission diagram
correspond-ing to the dipolar emission in far field for all the experimental conditions. By analyzcorrespond-ing the
emission^{0}s polarization together with the emission pattern, I could accurately determine the
three-dimensional orientation of an emitting dipole.

To build-in the experiment setup following the proposed model, I did firstly replacement of the sample by a well-determined polarized laser light, checking the optical function of necessary components such as the dichroic, the halfwave plate, the prism, etc. in the whole system to get the best and most facile conditions for measurement. The remarkable result obtained is that I could determine the dipolar orientation of a nanoemitter within 5% uncertainty. On the other hand, we succeed in conjugating the back focal plane onto the EM-CCD camera in order to image the emission pattern. By analyzing the emission pattern of the nanoemitter, we have a complementary method to estimate the dipolar dimensionality. Then the orientation of the

Finally, I applied this combining method to investigate the semiconductor CdSe*/*CdS
nanoplatelets with different geometric structures: thin square platelets, thin rectangular platelets,
and cubic platelets. The agreement between the experimental data and the calculated
simu-lation confirms the relevance of the method. I also established a resimu-lationship between the
geometric structures of the platelets and the dipolar dimensionality and orientation of their
associated emitting dipoles. For cubic CdSe*/*CdS nanoplatelets, we observed two different
kinds of the dipolar orientation, parallel and perpendicular to the surface of the substrate.

This is a good and promising case to develop the efficient combination of nanoemitter with nanoantennas.

For future works, the more kinds of geometric structures would be utilized to complete our theoretical explanation. Moreover, unlike the spherical CdSe nanocrystal which is weakly polarized and lack of defined orientation when locating on a substrate, the cubic nanoplatelets stayed on its side face with an emitting dipole oriented vertical to the substrate could be an interesting topic for the efficient coupling with next generation nanoantennas.

**The polarization effect of the**

**retardation induced by the setup**

*θ*
z

x

y Θ

Φ d

k

O*ϕ*
*θ*

Φ d

*ϕ*
*ϕ*
*ϕ*
O*ϕ*

*FIGURE A.1: Schemetic of an one dimensitional dipole with its orientation along* *d~which is*
*defined as (*Θ*,*Φ*) and the propagation vector* *~k* *which is described by (θ*_{1}*, φ) in* *xyz* *reference*
*coordinates.*

In the *xyz* reference coordinates, we will consider an one dimensitional emitting dipole
(Figure A.1) which is oriented with an out-plane angle Θ relative to the *z* axis (the polar
angle) and an in-plane Φ relative to the *x* axis (the azimuthal angle) with the unit vector *u~** _{s}*
and

*u~*

*along two orgothonal direction of polarization, respectively. These two unit vectors are perpendicular to the propagation vector*

_{p}*~k*defined by a polar angle

*θ*

_{1}and an azimuthal angle

*~*

The corresponding unit vectors *v~** _{s}* and

*v~*

*of the transmitted beam after passing through the setup (the output) will be thus defined as:*

_{p}*~*

oil objective oil objective air objective air objective oil objective

*d*

*FIGURE A.2: (a) Schematic of the five cases corresponding to different experimental *
*configu-rations between the sample and the objective, numbered from (i) to (v) withd* *being the distance*
*from an emitter to the medium interface,* *n*_{1} *denoting the index of the medium containing the*
*emitter, and* *n*_{2} *for the index of the other medium: (i) emitters in an homogeneous medium*
*of* *n*_{1}*; (ii) emitters on a planar substrate of index* *n*_{1} *and covered by a polymer layer with a*
*thickness* *d* *of the same index while the upper medium of index* *n*_{2} *< n*_{1}*; (iii) emitters at a*
*distance d (with d tending towards 0) from a substrate with an index* *n*_{2} *without any protecting*
*layer while* *n*_{1} = 1 *and (iv) emitters on a planar substrate with a polymer protecting layer of*
*index* *n*_{1} *while* *n*_{2} = 1*; (v) emitters in the medium of index* *n*_{1} *(as deposited at a distance* *d*
*(with* *d* *tending towards 0) from a planar surface without the covering layer), observed by an*
*oil objective of index* *n*_{2} *> n*_{1} *[27].*

The expression of the electrical field of the beam exiting the setup is extracted from the thesis of Clotile Lethiec [27] for reflection configuration (ii) and (iii) schematized in Figure A.2

as the followings:
The emitting power collected after placing a polarizer with a rotating angle of*β* after the
microscopy is also taken as:

*P*(*β*) = ^{Z} ^{θ}^{1}^{max}

with *ψ* denoting the retardation induced by the setup.

We have:

= *sin*Θ

2 *cosθ*_{1}(1−*r*_{p}*e** ^{i∆}*) (

*cosβ*(

*cos*(Φ−2

*φ*) +

*cos*Φ) +

*e*

^{iψ}*sinβ*(−sin(Φ−2

*φ*) +

*sin*Φ)) (A.8)

Hence:

*P*(*β*) =*A sin*^{2}Θ +*B cos*^{2}Θ +*C sin*^{2}Θ|cosβ cosΦ +*e*^{iψ}*sinβ sin*Φ|^{2}

=*A sin*^{2}Θ +*B cos*^{2}Θ + *C*

2 *sin*^{2}Θ(1 +*cos*2*β cos*2Φ +*sin*2*β sin*2Φ*cosψ*) (A.9)
with

*A*=^{Z} ^{θ}^{1max}

*θ*1=0

*D*^{2} *π*

4*n*_{1}|(1 +*r*_{s}*e** ^{i∆}*)−

*cosθ*

_{1}(1−

*r*

_{p}*e*

*)|*

^{i∆}^{2}

*sinθ*

_{1}

*dθ*

_{1}(A.10)

*B* =^{Z} ^{θ}^{1}^{max}

*θ*1=0

*D*^{2}*π n*_{1}|1 +*r*_{p}*e** ^{i∆}*)|

^{2}

*sin*

^{3}

*θ*

_{1}

*dθ*

_{1}(A.11)

*C* =^{Z} ^{θ}^{1max}

*θ*1=0

*D*^{2} *π*

2 *n*_{1}|1 +*r*_{s}*e** ^{i∆}*+

*cosθ*

_{1}(1−

*r*

_{p}*e*

*)|*

^{i∆}^{2}

*sinθ*

_{1}

*dθ*

_{1}(A.12) We define the measured value Φ

*mes*as:

*tan*2Φ*mes* =*tan*2Φ*cosψ* (A.13)

Therefore, Equation A.9 becomes

*P*(*β*) =*A sin*^{2}Θ +*B cos*^{2}Θ + *C*

2 *sin*^{2}Θ(1 + *cos*2Φ
*cos*2Φ*mes*

*cos*(2(*β*−Φ*mes*)) (A.14)
The degree of polarization is thus written as:

*δ** _{mes}* =

*P*

*−*

_{max}*P*

_{min}*P** _{max}*+

*P*

*=*

_{min}*Csin*

^{2}(Θ)

(2*A*−2*B* +*C*)*sin*^{2}(Θ) + 2*B*

*cos*2Φ

*cos*2Φ*mes* (A.15)
Finally, we conclude the relationship between *δ** _{mes}* (the degree of polarization measured
from the experiments by the realistic setup with a retardation of

*ψ*) and

*δ*(Θ) (the actual degree of polarization of the emission from the dipole (the actual value we would obtain with a setup

without any retardation effect):

*δ** _{mes}* =

*δ*(Θ)

*cos*2Φ

*cos*2Φ

*mes*

(A.16) These calculations could be applicable for the configuration (iv). The configuration (v) is more complicated and will not be treated here. The relation A.13 and A.16 can be as well straightforwardly applied to the case of a two dimensional dipole.

[1] C. J. Chunnilall, I. P. Degiovanni, S. Kuck, I. Muller, and A. G. Sinclair. Metrology of
single-photon sources and detectors: a review. *Optical Engineering*, 53(8):081910, 2014.

[2] A. Kuhn and D. Ljunggren. Cavity-based single-photon sources.*Contemp. Phys.*, 51:289–

313, 2010.

[3] T. E. Northup and R. Blatt. Quantum information transfer using photons. *Nat. Photon.*,
8:356–363, 2014.

[4] A. F. Koenderink, A. Alu, and A. Polman. Nanophotonics: shrinking light-based
tech-nology. *Science*, 348(6234):516–521, 2015.

[5] Z. H. Peng, S. E. de Graaf, J. S. Tsai, and O. V. Astafiev. Tuneable on-demand
single-photon source in the microwave range. *Nat. Commun.*, 7:12588, 2016.

[6] I. Aharonovich, D. Englund, and M. Toth. Solid-state single-photon emitters. *Nat.*

*Photon.*, 10(10):631–641, 2016.

[7] T. Grange, G. Hornecker, D. Hunger, J. P. Poizat, J. M. Gérard, P. Senellart, and A.
Auf-feves. Cavity-funneled generation of indistinguishable single photons from strongly
dissi-pative quantum emitters. *Phys. Rev. Lett.*, 114(19):193601–193606, 2015.

[8] A. G. Curto, G. Volpe, T. H. Taminiau, M. P. Kreuzer, R. Quidant, and N. F. van
Hulst. Unidirectional emission of a quantum dot coupled to a nanoantenna. *Science*,
329(5994):930–933, 2010.

[9] W. H. P. Pernice, C. Schuck, O. Minaeva, M. Li, G.N. Goltsman, A.V. Sergienko, and H.X.

Tang. High-speed and high-efficiency travelling wave single-photon detectors embedded
in nanophotonic circuits. *Nat. Commun.*, 3:1325, 2012.

[10] Y. M. He, Y. He, Y. J. Wei, D. Wu, M. Atature, C. Schneider, S. Hofling, M. Kamp,
C. Y. Lu, and J. W. Pan. On-demand semiconductor single-photon source with near-unity
indistinguishability. *Nat. Nano.*, 8(3):213–217, 2013.

[11] T. B. Hoang, G. M. Akselrod, and M. H. Mikkelsen. Ultrafast room-temperature single
photon emission from quantum dots coupled to plasmonic nanocavities. *Nano Lett.*,
16(1):270–275, 2016.

[12] M. K. Akhlaghi, E. Schelew, and J. F. Young. Waveguide integrated superconducting
single-photon detectors implemented as near-perfect absorbers of coherent radiation. *Nat.*

*Commun*, 6:8233, 2015.

[13] M. Gaio, M. Moffa, M. Castro-Lopez, D. Pisignano, A. Camposeo, and R. Sapienza.

Modal coupling of single photon emitters within nanofiber waveguides. *ACS Nano*,
10(6):6125–6130, 2016.

[14] , K. Słowik, J. Straubel, F. Lederer, R. Filter and Carsten Rockstuhl. Nanoantennas for
ultrabright single photon sources. *Opt. Lett.*, 39(5):1246–1249, 2014.

[15] J. Straubel, R. Filter, C. Rockstuhl, and K. Słowik. Plasmonic nanoantenna based
trig-gered single-photon source. *Phys. Rev. B.*, 93(19):195412–195423, 2016.

[16] C. Belacel, B. Habert, F. Bigourdan, F. Marquier, J. P. Hugonin, S. Michaelis de
Vas-concellos, X. Lafosse, L. Coolen, C. Schwob, C. Javaux, B. Dubertret, J. J. Greffet,
P. Senellart, and A. Maitre. Controlling spontaneous emission with plasmonic optical
patch antennas. *Nano Lett.*, 13(4):1516–1521, 2013.

[17] L. Novotny and N. van Hulst. Antennas for light. *Nat. Photon.*, 5(2):83–90, 2011.

[18] F. Bigourdan, J. Paul. Hugonin, F. Marquier, C. Sauvan, and J. J. Greffet. Nanoantenna
for electrical generation of surface plasmon polaritons. *Phys. Rev. Lett.*, 116(10):106803–

106808, 2016.

[19] L. Lin and Y. Zheng. Optimizing plasmonic nanoantennas via coordinated multiple
coupling. *Scientific Reports*, 5:14788, 2015.

[20] D. Vercruysse, Y. Sonnefraud, N. Verellen, F. B. Fuchs, G. Di Martino, L. Lagae, V. V.

Moshchalkov, S. A. Maier, and P. Van Dorpe. Unidirectional side scattering of light by a
single-element nanoantenna. *Nano Lett.*, 13(8):3843–3849, 2013.

[21] N. Liu, M. L. Tang, M. Hentschel, H. Giessen, and A. P. Alivisatos.
Nanoantenna-enhanced gas sensing in a single tailored nanofocus. *Nat. Mater.*, 10(8):631–636, 2011.

[22] Y. Kim, C. Ippen, T. Greco, M. S. Oh, C. J. Han, J. Lee, A. Wedel, and J. Kim.

Semitransparent quantum dot light-emitting diodes by cadmium-free colloidal quantum
dots. *J. Nanosci. Nanotechnol.*, 14(11):8636–8640, 2014.

[23] J. Q. Grim, L. Mannaab, and I. Moreels. A sustainable future for photonic colloidal
nanocrystals. *Chem. Soc. Rev.*, 44:5897–5914, 2015.

[24] M. Holzinger, A. Le Goff, and S. Cosnier. Nanomaterials for biosensing applications: a
review. *Front. Chem.*, 2:63, 2014.

[25] S. Roy and Z. Gao. Nanostructure-based electrical biosensors. *Nanotoday*, 4(4):318–334,
2009.

[26] A. Dousse, L. Lanco, J. Suffczynski, E. Semenova, A. Miard, A. Lemaitre, I. Sagnes, C.

Roblin, J. Bloch, and P. Senellart. Controlled light-matter coupling for a single quantum
dot embedded in a pillar microcavity using far-field optical lithography. *Phys. Rev. Lett.*,
101(26):267404, 2008.

[27] C. Lethiec. Emission polarisee de nanoemetteurs; excitation de plasmons sur une surface
metallique. *PhD Thesis of Pierre and Marie Curie University (University of Paris VI).*,
2014.

[28] S. Ithurria, M. D. Tessier, B. Mahler, R. P. S. M. Lobo, B. Dubertret, and A. L. Efros.

Colloidal nanoplatelets with two-dimensional electronic structure. *Nat. Mater.*, 10:936–

941, 2011.

[29] Z. Li, H. Qin, D. Guzun, M. Benamara, G. Salamo, and X. Peng. Uniform thickness and colloidal-stable cds quantum disks with tunable thickness: Synthesis and properties.

*Nano Research*, 5(5):337–351, 2012.

[30] J. S. Son, K. Park, S. G. Kwon, J. Yang, M. K. Choi, J. Kim, J. H. Yu, J. Joo, and
T. Hyeon. Dimension-controlled synthesis of cds nanocrystals: from 0d quantum dots to
2d nanoplates. *Small*, 8(15):2394–2402, 2012.

[31] R. Benchamekh, N. A. Gippius, J. Even, M. O. Nestoklon, J. M. Jancu, S. Ithurria, B.

Dubertret, A. L. Efros, and P. Voisin. Tight-binding calculations of image-charge effects
in colloidal nanoscale platelets of cdse. *Phys. Rev. B.*, 89(3):035307–035314, 2014.

[32] C. Bouet, M. D. Tessier, S. Ithurria, B. Mahler, B. Nadal, and B. Dubertret. Flat colloidal
semiconductor nanoplatelets. *Chem. Matter.*, 25(8):1262–1271, 2013.

[33] Marvin Minsky. Memoir on inventing the confocal scanning microscope. *Scanning*,
10(4):128–138, 1988.

[34] C.A. Gehring, D. A. Williams, S. H. Cody, and R. W. Parish. Phototropism and
geotropism in maize coleoptiles are spatially correlated with increases in cytosolic free
calcium. *Nature*, 345(6275):528–530, 1990.

[35] T. R. Corle and G. S. Kino. Confocal scanning optical microscopy and related imaging
systems. *New York: Academic Press*, 1996.

[36] H. Bach, A. Renn, and U. P. Wild. Spectral imaging of single molecules. *Single Mol.*,
1(1):73–77, 2000.

[37] E. J. G. Peterman, H. Sosa, and W. E. Moerner. Single-molecule fluorescence spectroscopy
and microscopy of biomolecular motors. *Ann. Rev. Phys. Chem.*, 55:79–96, 2004.

[38] P. Bharadwaj, B. Deutsch, and L. Novotny. Optical antennas. *Adv. Opt. Photonics*,
1(3):438–483, 1996.

[39] T. V. Raziman and O. J. F. Martin. Orientation dependence of plasmonically enhanced
spontaneous emission. *J. Phys. Chem. C*, 120(37):21037–21046, 2016.

[40] X. Brokmann, M. V. Ehrensperger, J. P. Hermier, A. Triller, and M. Dahan. Orientational
imaging and tracking of single cdse nanocrystals by defocused microscopy. *Chem. Phys.*

*Lett.*, 406(1-3):210–214, 2005.

[41] J. J. Macklin, J. K. Trautman, T. D. Harris, and L. E. Brus. Imaging and time-resolved
spectroscopy of single molecules at an interface. *Science*, 272(5259):255–258, 1996.

[42] C. Vion, P. Spinicelli, L. Coolen, C. Barthou, J.M. Frigerio, J.P. Hermier, and A. Maitre.

Controlled modification of single colloidal cdse/zns quantum dots fluorescence through
interactions with gold surface plasmons. *Opt. Express*, 18(7):7440–7455, 2010.

[43] A. Badolato, K. Hennessy, M. Atature, J. Dreiser, E. Hu, P. M. Petroff, and A. Imamoglu.

Deterministic coupling of single quantum dots to single nanocavity modes. *Science*,
308(5725):1158–1161, 2005.

[44] O. Gazzanov, S. Michaelis de Vasconcellos, K. Gauthron, C. Symonds, J. Bloch, P. Voisin, J. Bellessa, A. Lemaitre, and P. Senellart. Evidence for confined tamm plasmon modes under metallic microdisks and application to the control of spontaneous optical emission.

*Phys. Rev. Lett.*, 107(24):247402–247407, 2011.

[45] K. Hennessy, C. Hoogerle, E. Hu, A. Badolato, and A. Imamoglu. Tuning photonic
nanocavities by atomic force microscope nano-oxidation. *Appl. Phys. Lett.*, 89(4):041118–

041121, 2006.

[46] F. Pagliano, Y. J. Cho, T. Xia, F. van Otten, R. Johne, and A. Fiore. Dynamically
controlling the emission of single excitons in photonic crystal cavities. *Nature *
*Communi-cations*, 5:5786/1–6, 2014.

[47] X. Brokmann, M. V. Ehrensperger, J. P. Hermier, A. Triller, and M. Dahan. Orientational
imaging and tracking of single cdse nanocrystals by defocused microscopy. *Chem. Phys.*

*Lett.*, 406(1-3):210–214, 2005.

[48] E. Toprak, J. Enderlein, S. Syed, S. A. McKinney, R. G. Petschek, T. Ha, Y. E. Goldman,
and P. R. Selvin. Defocused orientation and position imaging (dopi) of myosin v. *Proc.*

*Natl. Acad. Sci. U.S.A.*, 103(17):6495–6499, 2006.

[49] A. P. Bartko and R. M. Dickson. Imaging three-dimensional single molecule orientations.

*J. Phys. Chem. B*, 103(51):11237–11241, 1999.

[50] S. A. Empedocles, R. Neuhauser, and M. G. Bawendi. Three-dimensional orientation
measurements of symmetric single chromophores using polarization microscopy. *Nature*,
399:126–130, 1999.

[51] J. T. Fourkas. Rapid determination of the three-dimensional orientation of single
molecules. *Opt. Lett.*, 26(4):211–213, 2001.

[52] C. Lethiec, J. Laverdant, H. Vallon, C. Javaux, B. Dubertret, J. M. Frigerio, C. Schwob, L.

Coolen, and A. Maitre. Measurement of three-dimensional dipole orientation of a single
fluorescent nanoemitter by emission polarization analysis. *Phys. Rev. X*, 4(2):021037–

021049, 2014.

[53] T. Ha, Th. Enderle, D. S. Chemla, P. R. Selvin, and S. Weisss. Single molecule dynamics
studied by polarization modulation. *Phys. Rev. Lett.*, 77(19):3979–3982, 1996.

[54] D. Goorskey, M. Xiao, Z. A. Peng, X. Chen, A. Nazzal, and X. Pengi. Polarization
spectroscopy of single cdse quantum rods. *Phys. Rev. B*, 64(24):245304–245308, 2001.

[55] P. Spinicelli, A. Fiore, J. P. Hermier, L. Manna, R. Cingolani, E. Giacobino, M. De Vittorio, F. Pisanello, L. Martiradonna, and A. Bramati. Dots-in-rods as polarized single

[55] P. Spinicelli, A. Fiore, J. P. Hermier, L. Manna, R. Cingolani, E. Giacobino, M. De Vittorio, F. Pisanello, L. Martiradonna, and A. Bramati. Dots-in-rods as polarized single